87

88

**Chapter 6 **

**Conclusion and future work **

In this last chapter a brief summary of this master thesis work needs to be carried out, in order to highlight the main aspects of the project.

*In the months spent at Politecnica de Madrid, the behaviour of composite materials used in *
naval field and subjected to water blast explosion was studied. First of all, a literature survey
was carried out, in order to better understand the importance of the goal of the project. In fact,
during the last years, several studies on these materials have been conducted. The behaviour
of these composite materials subjected to static, quasi-static and dynamic impact was deeply
studied, while there are not enough researches on the subjection to ballistic impacts. Materials
used in naval field must support several critical conditions, like thermal cycling, dynamic
loads and impulsive attacks among others. This led to the need pursued in this project.

In order to carry out this object, an experimental device, able to simulate a submarine mine, was designed based on the Hopkinson bar device. It was never used before and consists of the combination of an incident bar with an aluminium chamber. The incident bar was screwed to a piston (the frontal face of the box) and was hit by a projectile powered with compressed air.

The impact was converted in a plane wave in the water inside the aluminium box and it was this plane wave itself to hit the sample, fixed behind the aluminium box. The experimental device was also provided with an instrumental system which allowed to obtain experimental measures, like the deformation suffered by the sample and the pressure in the chamber.

The focus was on four FRP (fiber reinforced polymers) types made in vinylester reinforced with: carbon, glass, basalt-glass and carbon-glass. It means that it was studied not-hybrid and hybrid configuration. In the case of the hybrid configuration (two fiber types in the same panel), it was also considered the possible different behaviour if the test is conducted from the side of glass, or from the side of carbon and basalt. Another focus of this project was on the

89 study of the possible influence after the immersion in seawater. In fact, half samples were put in a bath of saltwater until the saturation level.

Another objective of this master thesis work was to develop an analytical model that allowed to predict the behaviour of composite materials subjected to water blast explosion. The analytical model was based on Vicente Sánchez’s equations and it was implemented on matlab. The input of the software was the pressure history obtained with experimental device and the output was a deformation archive calculated by the program. For each sample it was calculated the analytical deformation, in order to compare all the analytical and experimental results and to understand if the model would be reliable.

The experimental measures were analysed in order to compare all the conditions considered and to find the material that better behave in this application studied.

Regarding the hybrid materials, half of the specimens were tested in a side and half on the other side, but no appreciable differences were found, meaning that the hybrid composites behaved in the same way depending on the side involved in the impact. As regards the immersion in water, it was found that the deformations reached by saturated samples were very similar to the ones reached by dry specimens. It means that the immersion did not influence the behaviour of these composite materials.

It was also found that CFRP (carbon fiber reinforced polymer) is the composite type that behave worse of anyone. In fact, all the CFRP samples were broken after the tests and they showed the higher deformation values. Hybrid samples and especially carbon-glass showed the lowest deformation values, but it cannot be considered the best material in this application, because more than half specimens were delaminated after tests. Finally, GFRP (glass fiber reinforced polymer) were the only ones to not show any signs of damage after tests, therefore it can be concluded that they were the best materials for this application. It was also important to say that these conclusions can be applied just in the case of this project, meaning that a different, thickness, a different number of layers, a better homogeneous configuration of the fibers could led to different results. The reason behind the better behaviour of GFRP seems to be its higher compliance, which allows to reach higher deflection levels without compromising its integrity.

Regarding the analytical model, experimental and analytical deformation were compared, and it was found that analytical curves are very similar to experimental ones, especially for the peak values reached, which also is the most important parameter, because it represented the maximum deformation caused by the blast and, in principle, the highest stress levels for the

90 specimens. It can be concluded that analytical model is suitable for the prediction of the behaviour of composite materials subjected to submarine blast load.

Possible future works can be carried out. It can be conducted X-ray analysis to better evaluate the internal damage in the samples tested and to measure the residual stresses. It can be tested under different environmental conditions, such as different temperatures, considering that materials used in naval field can be subjected to thermal shock. Different thickness, number of layers, fibers disposition or, for example, a more homogeneous disposition of fibers in hybrid materials in order to confirm if the trends obtained in this work can be extrapolated to other configurations.

Moreover, it could be designed an improved experimental device based on that used in this project, considering that many difficulties slowed down the tests. However, the experimental device was been designed to study the behaviour of any type of material, therefore, in future can be used this device or another improved one to test different types of materials.

Finally, the analytical model predicted quite well the behaviour of the materials considered, then it can be used to study any type of materials, simply changing the input variables on the geometry and on the properties of the panel.

91

92

**Appendix**

**Matlab software **

*clear *

*%geometry and properties% *

*a=0.17; %dimension of the panel in m *
*b=0.225; %dimension of the panel in m *
*n=; %number of layers *

*S=; %cross-section area of the fiber *
*l=; %distance between fibers *
*E=; %Young Modulus in Pa *
*rho=; %Density in kg/m3 *

*sr=; %critical stress of the fiber in Pa *
*e=0.003; %thickness of the panel in m *
*mpiston=1.132+1.017; %piston mass *
*frozamiento=100; %friction *

*%select the pressure archive% *

*ruta='../Ensayos/SAMPLE/'; *

*input_presion='presion.csv'; *

*output_deflexion='deflexion'; *

*file=fopen([ruta,input_presion],'r');%pressure in MPa, time in s *
*P=csvread([ruta,input_presion]); *

*fclose(file); *

*%file_res=fopen([ruta,'Registro_proceso_calculo'],'w') *

*%fprintf(file_res,'Fecha %s\n',date) *

*%ITERATIVE PROCESS% *

*[f,c]=size(P); *

*tp=P(:,1);%time vector *
*p=P(:,2);%pressure vector *
*t(1)=0; *

*rhoH2O=1000; %Kg/m^3% *

*m=rho*e*a*b; *

*s(1)=0;%stress in the sample *

93
*v(1)=0;%panel speed *

*dv(1)=0; *

*y(1)=0.00001;%deflection *

*theta(1,1)=0.00001;%angle with normal to sample *
*theta(2,1)=0.00001; *

*fp(1)=p(1)*1e6*a*b;%pushing force *
*fr(1)=0;%resistant force *

*mH2O(1)=0;%mass of the water in the box *
*dmH2O(1)=0; *

*i=2; *

*x(1)=0; *

*sigma=s(1); *

*while(sigma<sr && i<=number of values in the pressure archive used) *
*dt(i-1)=tp(i)-tp(i-1); *

*t(i)=t(i-1)+dt(i-1); *

*[sol,niter]=newton_raphson_rectangular(@fun_rectangular,@dfun_rectangular,theta,a,b,y(i-1),1E-3); *

*theta(1,i)=sol(1); *

*theta(2,i)=sol(2); *

*epsx(i)=2*y(i-1)*(1-cos(sol(1)))/(sin(sol(1))*b *
*epsy(i)=(1/cos(sol(2)))-1 *

*x(i)=y(i-1)/theta(1,i); *

*s(i)=(theta(2,i)/abs(theta(2,i)))*E*((1/cos(theta(2,i)))-1); *

*fp(i)=p(i)*1E6*a*b; *

*fr(i)=s(i)*n*S*2*(a*sin(sol(1))+b*sin(sol(2)))/l *
*if (s(i)>s(i-1)) *

*mH2O(i)=rhoH2O*(0.5*a*b*y(i-1)-(1/3)*a*y(i-1)*x(i)); *

*dmH2O(i)=mH2O(i)-mH2O(i-1); *

*dv(i)=((fp(i)-fr(i))*dt(i-1)-dmH2O(i)*v(i-1))/(m+mH2O(i)); *

*else *

*mH2O=rhoH2O*0.2*0.25*0.15; *

*dv(i)=((fp(i)-fr(i))*dt(i-1))/(m+mH2O+mpiston+frozamiento); *

*end *

*v(i)=v(i-1)+dv(i); *

*dy(i)=v(i)*dt(i-1); *

*y(i)=y(i-1)+dy(i); *

*sigma=s(i); *

*i=i+1; *

*end *

*D=[t',1000*y'];%save the deflection in mm *
*csvwrite([ruta,output_deflexion],D); *

94

95

**References **

**References**

*[1] Badini C. (2013), Materiali compositi per l'ingegneria, Celid, 248 pp. *

*[2] Pagliara G., (n.d.), Compositi a matrice o a rinforzo ceramico, lezioni di tecnologia ceramica. *

*[3] Licciulli A (2009), Materiali compositi e loro rinforzi, Corso di scienza e ingegneria dei materiali, *
Università del Salento.

*[4] Anon (2012), Materiali compositi, dispense corsi di laurea a distanza, Scienza dei materiali, *
Politecnico di Torino.

*[5] Altervista (2011), Materiali Compositi. [online] disponibile a: *
<http://adpaloha.altervista.org/wp-content/uploads/2012/11/Materiali-Compositi_______.pdf> [Ultimo accesso 15/05/19].

*[6] Vannucci (2008), Cosa sono i materiali compositi, Capitolo 1, Dispense Scuola di dottorato di *
ingegneria, Università di Pisa.

*[7] Rossetti G., (n.d.), Progettazione con materiali, presentazione disponibile a: *

*<slideplayer.it/slide/13404486/> [ultimo accesso 21/11/19]. *

*[8] Octima, (2016), poliestere, vinilestere o epossidica, PDF disponibile a: *
<https://www.octima.it/wp-content/uploads/2016/01/09_Nau_Gurit.pdf>.

*[9] Marinò A. (2016), Costruzioni navali in composito, dispense, Università degli studi di Trieste. *

*[10] Albicini L. (2016), I materiali compositi avanzati (FRP-FRG). Classificazione e applicazioni nel *
*restauro e ricostruzione post-sisma, tesi di laurea, Scuola di ingegneria e architettura, Università di *
Bologna.

*[11] Fidia s.r.l. (n.d.), Tessuti in fibra naturale di basalto BFRP, disponibile a: *

<http://www.fidiaglobalservice.com/ita/tessuti_basalto.html> [ultimo accesso: 29/10/19].

*[12] Naik S., (2013), Stress wave propagation in split Hopkinson pressure bar, master thesis, *
department of civil engineering, National institute of technology Rourkela.

*[13] Mazón P., (2018), Estudio del comportamiento a impacto de alta velocidad en materiales *
*compuestos del sector naval, tesi di laurea, Department of material’s engineering, Politecnica de *
Madrid.

*[14] Mouritz A.P., Gargano A., Pingkarawat K., Das R., Pickerd V., Delaney T., (2017), Effect of *
**seawater on the explosive blast response of a carbon fiber laminate, 109 (A), 382-391. **

*[15] Arora H., Del Linz P., Dear J. (2017), Damage and deformation in composite sandwich panels *
**exposed to multiple and single explosive blasts, 104, 95-106. **

*[16] Dear J.P., Rolfe E., Kelly M., Hooper P.A., Arora H., (2016), X-Ray CT Analysis after Blast of *
**Composite Sandwich Panels, 167, 176-181. **

*[17] D’Angelo G., (2017/2018), High speed impact properties of composite materials, Department of *
management engineering, Università degli studi di Napoli Federico II.

*[18] Dhand V., Mittal G., Rhee K.Y., Park S., Hui D., (2015), A short review on basalt fiber *
**reinforced polymer composites, 73, 166-180. **

*[19] Linkedin, (2011), Composite materials, disponibile a: *

<https://player.slideplayer.com/12/3505368/data/images/img18.jpg>.